This guide has been prepared to assist welding personnel with the preparation of welding procedures required as part of their company certification to CSA Standards W47.1, W47.2 and W186.Descripción completa
General When structures and pressurised items are fabricated by welding, it is essential that all the welded joints are sound and have suitable properties for their application. application. Control of welding is achieved by means of Welding Procedure Specifications (WPSs) that give detailed written instructions about the welding conditions that must be used to ensure that welded joints have the required properties. Although WPSs are shop floor documents to instruct welders, welding inspectors need to be familiar with them because they will need to refer to WPSs when they are checking that welders are working in accordance with the specified requirements. Welders need to be able to understand WPSs, have the skill to make welds that are not defective and demonstrate these abilities before being allowed to make production welds.
Qualifi Qualifi ed Welding Procedure Specific ations It is industry practice to use qualified WPSs for WPSs for most applications. applications. A welding procedure is usually qualified by making a test weld to demonstrate that the properties of the joint satisfy the requirements specified by the application standard and the client/end user. Demonstrating Demonstrating the mechanical mechanical properties of the joint is the principal purpose of qualification tests, but showing that a defect-free weld can be produced is also very important. Production welds made in accordance with welding conditions similar to those used for a test weld should have similar properties and therefore be fit for their intended purpose. Figure 1 is an example of a typical WPS written in accordance with the European Welding Standard format giving details of all the welding conditions that need to be specified.
Welding Welding standards for procedure qualification European and American Standards have been developed to give comprehensive comprehensive details about: • • • •
How a welded test piece must be made to demonstrate joint properties. How the test piece must be tested. What welding details need to be included in a WPS. The range of production welding allowed by a particular qualification test weld.
The principal European Standards that specify these requirements are: EN ISO 15614 Specification and qualification of welding procedures for metallic materials – Welding procedure test Part 1: Part 2:
Arc and gas welding of steels and arc welding of nickel and nickel alloys Arc welding of aluminium and its alloys
The principal Am erican Standards for procedure qualification are:
ASME Secti on IX
Pressurised systems (vessels and pipework)
Structural welding of steels
Structural welding of aluminium
The qualification process for welding procedures Although qualified WPSs are usually based on test welds that have been made to demonstrate weld joint properties; welding standards also allow qualified WPSs to be written based on other data (for some applications). Some alternative ways that can be used for writing qualified WPSs for some applications are: • •
Qualification by adoption of a standard welding procedure – test welds previously qualified and documented by other manufacturers. Qualification based on previous welding experience – weld joints that have been repeatedly made and proved to have suitable properties by their service record.
Procedure qualification to European Standards by means of a test weld (and similar in ASME Section IX and AWS) requires a sequence of actions that is typified by those shown by Table 1. A successful procedure qualification test is completed by the production of a Welding Procedure Qualification Record (WPQR), an example of which is shown by Figure 2.
Relation ship between a WPQR and a WPS Once a WPQR has been produced, the welding engineer is able to write qualified WPSs for the various production weld joints that need to be made. The welding conditions that are allowed to be written on a qualified WPS are referred to as the qualification range and this range depends on the welding conditions used for the test piece (the as-run details) and form part of the WPQR. Welding conditions are referred to as welding variables by European and American Welding Standards and are classified as either essential or nonessential variables. These variables can be defined as follows: •
Essential variable: A variable that has an effect on the mechanical properties of the weldment (and if changed beyond the limits specified by the standard will require the WPS to be re-qualified). Non-essential variable: A variable that must be specified on a WPS but does not have a significant effect on the mechanical properties of the weldment (and can be changed without need for re-qualification but will require a new WPS to be written).
It is because essential variables can have a significant effect on mechanical properties that they are the controlling variables that govern the qualification range and determine what can be written in a WPS. If a welder makes a production weld using conditions outside the qualification range given on a particular WPS, there is danger that the welded joint will not have the required properties and there are then two options: 1 Make another test weld using similar welding conditions to those used for the affected weld and subject this to the same tests used for the relevant WPQR to demonstrate that the properties still satisfy specified requirements. 2 Remove the affected weld and re-weld the joint strictly in accordance with the designated WPS. Most of the welding variables that are classed as essential are the same in both the European and American Welding Standards but their qualification ranges may differ. Some application standards specify their own essential variables and it is necessary to ensure these are taken into consideration when procedures are qualified and WPSs written.
Examples of essential variables (according to European Welding Standards) are given in Table 2.
Welder Qualification The use of qualified WPSs is the accepted method for controlling production welding but this will only be successful if the welders are able to understand and work in accordance with them. Welders also need to have the skill to consistently produce sound welds (free from defects). Welding Standards have been developed to give guidance on what particular test welds are required in order to show that welders have the required skills to make particular types of production welds in particular materials.
Welding standards for welder qualification The principal European Standards that specify requirements are: EN 287-1
Qualification test of welders – Fusion welding Part 1: Steels
EN ISO 9606-2
Qualification test of welders – Fusion welding Part 2: Aluminium and aluminium alloys
Welding personnel – Approval testing of welding operators for fusion welding and resistance weld setters for fully mechanised and automatic welding of metallic materials
The principal Am eri can Standar ds that specify requirements for welder qualification are: ASME Sect io n IX Pressurised systems (vessels & pipework)
Structural welding of steels
Structural welding of aluminium
The qualification process for welders Qualification testing of welders to European Standards requires test welds to be made and subjected to specified tests to demonstrate that the welder is able to understand the WPS and to produce a sound weld. For manual and semi-automatic welding the emphasis of the tests is to demonstrate the ability to manipulate the electrode or welding torch.
For mechanised and automatic welding the emphasis is on demonstrating that welding operators have the ability to control particular types of welding equipment. American Standards allow welders to demonstrate that they can produce sound welds by subjecting their first production weld to NDT. Table 3 shows the steps required for qualifying welders in accordance with European Standards. Figure 3 shows a typical Welder Qualification Certificate in accordance with European Standards.
Welder qualification and produ ction welding allowed The welder is allowed to make production welds within the range of qualification recorded on his Welder Qualification Certificate. The range of qualification is based on the limits specified by the Welding Standard for welder qualification essential variables s – defined as: A var iable th at if ch anged beyon d th e limi ts sp ecifi ed by th e Weldin g Standard may require greater skill t han has been demonst rated by the test weld. Some welding variables that are classed as essential for welder qualification are the same types as those classified as essential for welding procedure qualification, but the range of qualification may be significantly wider. Some essential variables are specific to welder qualification. Examples of welder qualification essential variables are given in Table 4.
Period of validity for a welder qualification certificate A welder’s qualification begins from the date of welding of the test piece. The European Standard allows a qualification certificate to remain valid for a period of two years, provided that: • •
The welding co-ordinator, or other responsible person, can confirm that the welder has been work ing with in the initi al range of qualific ation. Working within the initial qualification range is confirmed every six months.
Prolongation of welder qualification A welder’s qualification certificate can be prolonged every two years by an examiner/examining body but before prolongation is allowed certain conditions need to be satisfied: • •
Records/evidence are available that can be traced to the welder and the WPSs used for production welding. Supporting evidence must relate to volumetric examination of the welder’s production welds (RT or UT) on two welds made during the six months prior to the prolongation date. Supporting evidence welds must satisfy the acceptance levels for imperfections specified by the European welding standard and have been made under the same conditions as the original test weld.
Table 1 Typical sequence for welding procedure qualification by means of a test weld The w welding e engineer wr ites a a p r el i m i n ar y Welding P Pr ocedur e S Specif ication r y W (pWPS) f f or each ttest c coupon tto b be w welded.
A welder makes the test coupon in accordance with the pWPS A welding inspector records all the welding conditions used to make the test coupon (called the as-run conditions).
An iindependent e examiner /examining b body/thir d p par ty iinspector m ay b r equested b e r to m monitor the p pr ocedur e q qualif ication.
The ttest c coupon iis s sub je accor dance w with tthe m methods s specif ied b by jected tto NDT iin a the S Standar d – visual iinspection, M MT o r P PT a and R RT o r UT.
The test coupon is destructively tested (tensile, bend, macro tests). The code/application standard client may require additional tests such as hardness, impact or corrosion tests – depending on material and application.
A Weldin g Pro cedur e Qualif ic ati on Record (WPQR) is pr epared by th e welding engineer giving d etails of: – As-run welding conditions – Results of the NDT – Results of the destructive tests – Welding conditions allowed for production welding If a third party inspector is involved he will be requested to sign the WPQR as a true record of the test.
Range for procedure qualification No range – process qualified must be used in production. Joints tested after PWHT and only qualify PWHT production joints. Joints tested as-welded only qualify as-welded production joints. Parent materials of similar composition and mechanical properties are allocated the same Material Group No; qualification only allows production welding of materials with the same Group No. Consumables for production welding must have the same European designation – as a general rule. A thickness range is allowed – below and above the test coupon thickness. AC only qualifies for AC; DC polarity (+ve or -ve) cannot be changed; pulsed current only qualifies for pulsed current production welding. The preheat temperature used for the test is the minimum that must be applied. The highest interpass temperature reached in the test is the maximum allowed. When impact requirements apply maximum HI allowed is 25% above test HI. When hardness requirements apply minimum HI allowed is 25% below test HI.
Table 3 The stages for qualification of a welder The welding engineer writes a WPS for welder qualification test piece.
The welder makes the test weld in accordance with the WPS A welding inspector monitors the welding to ensure that the welder is working in accordance with the WPS.
An independent examiner/examining body/third party inspector may be requested to monitor the test.
The test coupon is subjected to NDT in accordance with the methods specified by the Standard (visual inspection, MT or PT and RT or UT) For certain materials, and welding processes, some destructive testing may be required (bends or macros).
A welder’s Qualification Certificate is prepared showing the welding conditions used for the test piece and the range of qualification allowed by the Standard for production welding. If a third party is involved, the Qualification Certificate would be endorsed as a true record of the test.
Range for welder qualification No range – process qualified is process that a welder can use in production. Butt welds cover any type of joint except branch welds. Fillet welds only qualify fillets. Parent materials of similar composition and mechanical properties are allocated the same Material Group No; qualification only allows production welding of materials with the same Group No. but the Groups allow much wider composition ranges than the procedure Groups. Electrodes and filler wires for production welding must be of the same form as the test (solid wire, flux-cored etc); for MMA coating type is essential. A thickness range is allowed; for test pieces above 12mm allow ≥ 5mm. Essential and very restricted for small diameters: Test pieces above 25mm allow ≥ 0.5 x diameter used (minimum 25mm). Position of welding very important; H-L045 allows all positions (except PG).
Figure 1 Example of a Welding Procedure Specification (WPS) to EN 15614 format.